198 tD. von Aubel on the Influence of Magnetism 



Table [continued). 



(c) Alloys with Tin (cont.). 

 (2) Rods tempered. 





Temp. 



W, Wm. 



Trommsdorff bismuth, i 



absolutely pure. \ 



0-39 gr. tin to 100 gr. Bi. 1 



Sobering bismuth. 

 0-40 gr. tin to 100 gr. Bi. 1 



Trominsdorff bismuth I. J 

 0-46 gr. tin to 100 gr. Bi. 1 



Trominsdorff bismuth II. J 

 0-46 gr. tin to 100 gr. Bi. 1 



18-6 

 416 

 70-4 



16-6 

 41-8 

 73-9 



20-4 

 42-8 

 69-6 



24-5 

 40-6 



77-8 



0-2133 0-2136 

 0-2173 0-2178 

 02213 02213 



0-2100 0-2105 

 0-2145 0-2150 

 0-2148 02150 



01443 01443 

 0-1478 01478 

 0-1498 0-M98 



01529 01534 

 01554 0-1561 

 0-1574 01574 



(cl) Alloys with Lead. 

 (1) Rods slowly cooled. 



Trominsdorff bismuth, 1 



absolutely pure. < 



0-52 gr. Pb to 100 gr. Bi. [ 



Trominsdorff bismuth I. J 

 0-54 gr. Pb to 100 gr. Bi. 1 



Sobering bismuth. 

 0-49 gr. Pbto 100 gr. Bi. 1 



Trommsdorff bismuth II. J 



0-60 gr. Pb to 100 gr. Bi. 1 



1 



18-8 

 44-7 

 689 



21 



43-4 



71-6 



18-8 

 44-8 

 67-4 



15-4 



43 



69-8 



0-4925 

 0-4995 

 05015 



0-2713 

 0-2778 

 0-2878 



02631 

 0-2611 

 02620 



0-3923 



0-3878 

 0-3848 



0-4945 

 0-5015 

 0-5035 



0-2743 



0-2788 

 0-2888 



0-2656 

 0-2632 

 0-2630 



0-3963 

 0-3913 

 0-3871 



(2) Rods tempered. 



Trommsdorff bismuth, 1 



absolutely pure. \ 



0-52 gr. Pb to 100 gr. Bi. [ 



Trommsdorff bismuth I. 1 

 0-54 gr. Pb to lOOgr. Bi. 1 



Sohering bismuth. 

 0-49 gr. Pbto 100 gr. Bi. 1 



Trommsdorff bismuth II. J 

 0-60 gr. Pbto lOOgr. Bi. 1 



18-2 

 42-4 

 70-4 



174 



41-6 

 71 



18-8 

 44-4 

 70-2 



22-2 

 43-6 



72-2 



01690 



0-1725 

 01735 



00937 

 0-0929 

 0-0914 



0-1478 

 01458 

 01439 



01056 

 01056 

 01031 



0-1700 

 01730 



01735 



00947 

 00934 



U-0919 



01493 

 01468 

 01449 



0-1066 

 01061 

 01031 



